This practice covers procedures for making and curing cylinder and beam specimens from representative samples of fresh concrete for a construction project. C 31/C 31M Practice for Making and Curing Concrete Test 1 This test method is under the jurisdiction of ASTM Committee C09 on. Concrete. ASTM Standards: 2. C 31/C 31M Practice for Making and Curing Concrete Test. Specimens in the Field. C 42/C 42M Test Method for Obtaining and Testing .
|Published (Last):||17 July 2014|
|PDF File Size:||14.44 Mb|
|ePub File Size:||17.45 Mb|
|Price:||Free* [*Free Regsitration Required]|
Concrete cylinder samples are made for your lab technician to break in a hydraulic press machine and find the compressive strength of the concrete that is being poured for a specific part of a structure. You will get a representative sample of freshly mixed concrete from the truck or mixer, perform slump, temperature, and air content tests on it, and then make cylinders that will be taken back to the lab.
These samples provide quality control for architects and engineers and allow them to determine if they will be able to put that concrete into service for their structure, or if they need to remove what they have poured.
While you are out there making cylinders you can keep lookout for errors in the mixing and pouring of the concrete; field techs are expected to report things that go wrong to the site superintendent or project 31. The curing process will also help those in charge of the project determine how to best protect the concrete in the structure as it cures and gives them a set of limits for form and shoring removal time. Rods – 6×12 cylinders need the large tamping rod and 4×8 cylinders need the small tamping rod.
Please make sure your rods are clean and have a smooth hemispherical atsm before use, as specified in ASTM C Rodding is only used zstm the slump is greater or v to one inch; if the mix is very dry and the slump comes out to less aatm an inch you will have to vibrate the concrete to consolidate it thoroughly. Cylinder molds — These can be plastic or steel, but we typically use plastic molds. If steel molds are used, mineral oil will also be needed to lightly 311m the inside surface of the mold and keep the concrete from sticking to the mold.
ASTM C31 / C31M – 18b Standard Practice for Making and Curing Concrete Test Specimens in the Field
Whichever mold you are using, they will need to be watertight and resistant to damage from tamping, as specified in ASTM C Disposable molds are to be calibrated every time a new lot arrives.
I qstm advise you to carry an extra set of each size of mold to every job, because you never know if you might be asked to make another set. Excessive concrete buildup can be removed from metal scoops and rods by soaking them in vinegar overnight, then washing them off with soap and water and coating them with mineral oil to protect the galvanization. Wheelbarrow — Should be able to hold at least 1 31, foot of concrete, the minimum size required for concrete strength testing specimens.
Bucket of Water and Rag — Please clean off your equipment after each use to help keep it in spec. You can typically get water from a hose on the side of the concrete truck, or you could possibly bring your own water in a sealed container.
It is very important for the integrity of any test to have clean, working equipment. Vibrator optional — Should be internal and operate at a frequency of at least vibrations per minute.
The cylinder diameter needs to be at least 3 times as wide as the largest piece of aggregate the nominal aggregate sizeso we only make 4x8s when the nominal aggregate size is less than 1. Sample the concrete in accordance with ASTM C, making sure to mix your concrete sample thoroughly. The ultimate goal of the sampling process is to have a sample that is an average representation of what is going into the pour, to get the most accurate strength value in the lab.
When you sample the concrete, try to get your sample from the middle of the batch and not the first or last clumps of concrete, because the first or last portions may come out of the mixer slightly different from the rest of the batch. Ask if all water has been added before you get your sample, and also make sure you get the batch ticket from the driver of the truck, because you will need it later on when you are entering the sample into your computer system or otherwise filling out paperwork.
Batch tickets contain lots of useful information, like which mix design is being used on that pour and how long it aetm been since the truck left the plant it is recommended that concrete that has atm out more than 90 minutes should not be used in a pour, because concrete will start to harden up and be very difficult to pour evenly.
If you are making multiple sets of cylinders with more than one truck, write the number on the 311m ticket and on your paperwork so you know which truck goes with which set of cylinders. If you are also doing slump, temperature, and air content on this sample, note that you must have these cylinders made within 15 minutes of receiving the sample, so plan astj and set up your work area beforehand ASTM C Paragraph 4. It helps to group your equipment by test, so you have everything you need for each test in one place.
When you are picking a place to make your cylinders, make sure it is in a level area that is free of debris, away from vibration, and away from moving vehicles and large construction equipment. Be sure to write on your paperwork which location you are making or leaving your cylinders at, because someone else may be the one to come pick them up.
If you are rodding the cylinders to consolidate them, the amount of layers will vary by sample size: All cylinders in a set should be started at the same time and have their layers added at the same time you do not add three layers for one and then move on to the next cylinder, they must all have their first layer added and rodded before you move on to layer 2.
For both sizes, each layer will be rodded 25 times in an even pattern, distributing the holes uniformly over the cross-section of the mold. The bottom layer must be penetrated to the bottom of the mold, and for the layers above it you must go through that layer and about an inch into the layer below it.
When you are doing the last layer, if your mold is underfilled asstm can add extra concrete to keep it properly filled as you rod. After you rod each layer you need to tap the outside of your mold with an open hand about 10 to 15 times plastic molds may be damaged if you use a mallet to let excess air out of the cylinder and close the holes from rodding ASTM C31 Paragraph 9.
If you are vibrating the cylinders to consolidate them, you f always have 2 equal layers to put into the mold, but for 4x8s you insert the vibrator one time per layer and for 6x12s you insert it twice per layer.
You will know when the vibration is done when the surface of the concrete is relatively smooth and air bubbles have stopped coming up to the top surface. After you have consolidated the concrete, you will need to strike off the concrete to provide a smooth surface.
Use a back-and forth left-to-right sawing motion, starting in the middle and working away from you, then come back to the middle and move the strike-off bar towards you, still performing the same sawing motion. If 311m are large holes in the end of the cylinder, your lab tech will have to grind it down or saw cut the end of the cylinder, so you want it to be smooth. Use your rag to clean around the rim of the mold, wiping away excess concrete from the edge but never touching the material inside the rim.
Label each cylinder mold with the project number, the date and time you made the cylinder, and the sample number. Knowing the time and date will be important for the lab tech to know when to break the cylinders. Having the right sample number and project will help the lab know which set is which, which can get confusing if there are many cylinders coming in at the same time, so please label them wstm Cover each cylinder with an appropriate sized cylinder bag and place it in a protected location free of vibration and disturbances.
Cylinders need to be picked up anywhere from 18 to 48 hours after they are made. Don’t leave them out there for a week and forget about them or your lab tech is going to be very confused when they look for cylinders to break and find an empty moisture room. They need time to cure under moist temperature-controlled conditions and they do not need to be overly exposed qstm the elements.
When transporting cylinders, you will want to make sure they don’t bounce around in the truck or fly out, so you should have 31n cushioned transport racks to hold them in.
ASTM C31 – Making and Curing Concrete Test Specimens in the Field
Keep them away from the sun as well, because it can affect their temperature and change the way they cure. Drive carefully, these are the only samples you’ve got. Once you’re back at the office, get the cylinders off of your truck and out of the transport racks, removing their bags. Set them on the floor or on the table, whichever you prefer, and grab a stripping asm looks like a t-shaped metal bar and a rubber mallet.
ASTM C31 – Making and Curing Concrete Test Specimens in the Field | Owlcation
To strip a cylinder, insert the stripping tool into the top of the mold in the gap between the concrete and the mold, and hammer it all the way to the bottom of the mold. You could also use an air compressor to remove the mold quickly, using something to create a small hole at the bottom of the mold and blowing air through that. Once the cylinder is out you will need to label it and check it in through whatever system you use we use Metafield.
After the cylinder has been picked up, checked ashm, and carefully labelled make sure you have the right sample number and date! Ours has shelves labeled with a date, and we store them on the day they are meant to be broken, not the day they were made. Typically for 6x12s we break 2 at the seven day mark and 2 ast, the 28 day mark and leave a spare cylinder to break on the 56 day mark if the cylinders have still failed to meet the required strength.
Once they are in the moisture room and in the system you are all done. How many inches are in one layer of a concrete test specimen? Sign in or sign up and post using a HubPages Network account. Comments are not for promoting your articles or other sites. Other product and company names shown may be trademarks of their respective owners. HubPages and Hubbers authors may earn revenue on this page based on affiliate relationships and advertisements with partners including Amazon, Google, and others.
To provide a better website experience, owlcation. Please choose which areas of our service asttm consent to our doing so.
Equipment Required for Making Concrete Cylinders Rods – 6×12 cylinders need the large tamping rod and 4×8 cylinders need the small tamping rod. Strike-off Bar — Must be clean and level and must have a flat and even plane surface. Step 2 If you are also doing slump, temperature, and air content on this sample, note that you must have these cylinders made within 15 minutes of receiving the sample, so plan accordingly and set up your work area beforehand ASTM C Paragraph 4.
This is used to prevent bots and spam. This is used to detect comment spam. This is used to provide data on traffic to our website, all personally identifyable data is anonymized.
ASTM C31 – Making & Curing Concrete Specimens in the Field
This is used to collect data on traffic to articles and other pages on our site. Unless you are signed in to a HubPages account, all personally identifiable information is aastm.
This service allows you to sign up for or associate a Google AdSense account with HubPages, so that you can earn money from ads on your articles. No data is shared unless you engage with this feature. Some articles have YouTube videos embedded in them. Some articles have Vimeo videos embedded 31j them. This is used for a registered author who enrolls in the HubPages Earnings program and requests to be paid via PayPal.
No data is shared with Paypal unless you engage with this feature.
You can use this to streamline signing up for, or signing in to your Hubpages account. No data is shared with Facebook unless you engage with this feature.